Controllable synthesis of flake-like Al-doped ZnO nanostructures and its application in inverted organic solar cells
© Fan et al; licensee Springer. 2011
Received: 8 May 2011
Accepted: 4 October 2011
Published: 4 October 2011
Flake-like Al-doped ZnO (AZO) nanostructures including dense AZO nanorods were obtained via a low-temperature (100°C) hydrothermal process. By doping and varying Al concentrations, the electrical conductivity (σ) and morphology of the AZO nanostructures can be readily controlled. The effect of σ and morphology of the AZO nanostructures on the performance of the inverted organic solar cells (IOSCs) was studied. It presents that the optimized power conversion efficiency of the AZO-based IOSCs is improved by approximately 58.7% compared with that of un-doped ZnO-based IOSCs. This is attributed to that the flake-like AZO nanostructures of high σ and tunable morphology not only provide a high-conduction pathway to facilitate electron transport but also lead to a large interfacial area for exciton dissociation and charge collection by electrodes.
KeywordsAl-doped ZnO inverted organic solar cell electrical conductivity morphology
In the recent years, much attention in development of inverted organic solar cells (IOSCs) has been focused on zinc oxide (ZnO) nanostructures as an electron transport layer (ETL), which is attributed to its excellent chemical and thermal stability, high electron mobility, and easy fabrication [1–3]. One of the most popular structures is indium tin oxide/nanostructured ZnO/active layer/molybdenum oxide (MoO3)/anode [1, 2, 4, 5]. In such IOSC devices, however, ZnO nanostructures still remain challenging. On the one hand, the electrical conductivity (σ) of ZnO nanostructures, which determines the characteristic of electron transfer, is still not high enough for IOSCs. For example, the short-circuit current density (J SC) of ZnO nanorod (NR)-based IOSCs was usually limited to a small range of 6.0 to 6.5 mA cm-2 under simulated 100 mW cm-2 (AM 1.5 G) solar irradiation , which blocks its practical application. On the other hand, the non-absorbing ZnO NR arrays, synthesized via hydrothermal method, are usually too densely packed, making for an insufficient polymer filling fraction, low photon absorption efficiency, and exciton dissociation into free carriers at a donor-acceptor site before recombining . Moreover, owing to the smaller interfacial area between the ZnO NRs and the active layer, the power conversion efficiency (PCE) of ZnO NR-based IOSCs is often lower than that based on nanoparticles . If disperse and ultrathin ZnO nanostructures can be achieved, it will facilitate electron transfer of IOSCs by increasing the interfacial area between ZnO nanostructures and the active layer .
Recently, many efforts had been also made to improve the σ of ZnO nanostructures by doping various chemical elements such as gallium (Ga) [4, 7, 8], indium , and aluminum (Al) [10, 11] into ZnO nanostructures. Among them, Al-doped ZnO (AZO) nanostructures are capable of reaching the highest σ without deterioration in optical transmission . Moreover, it had been reported that the J SC could be improved dramatically by a Ga-doped ZnO NRs, which can increase the σ of the ETL and decrease the series resistance (R S) of IOSCs. Hence, it is possible to increase the device performance by doping Al concentrations in ZnO nanostructures.
In this paper, we demonstrate the performance enhancement of the IOSCs based on the flake-like AZO nanostructures acting as an ETL and a possible electron acceptor. By doping and varying Al concentrations in a solution of 0.025 M zinc nitrate [Zn(NO3)2·6H2O] and hexamethylenetetramine (HMT), we obtained ultrathin flake-like AZO nanostructures of high σ and distinct morphology. Moreover, the morphology of flake-like AZO nanostructures, such as the density and the size, can occur to change with varying the Al concentrations. Compared with that of the un-doped ZnO NR-based IOSCs, the PCE of the optimized AZO-based IOSCs has a dramatic increase from 1.04% to 1.65%.
Results and discussion
Device performance parameters of the IOSCs and the corresponding electrical conductivity
J SC (mA cm-2)
V OC (V)
R S (Ω cm2)
8.2 × 10-5
3.2 × 10-4
4.4 × 10-4
5.1 × 10-4
For the convenience of comparison, the length of the AZO NFs is kept at approximately 100 nm. Clearly, devices with un-doped ZnO have a bad performance: J SC = 8.56 mA cm-2, open-circuit voltage (V OC) = 0.360 V, FF = 0.337, and a PCE of 1.04%. With doping 1 and 2 mM Al concentrations, the J SC of devices increases to 10.26 and 11.08 mA cm-2, and the PCE increases to 1.26% and 1.44%, respectively. With increasing Al concentrations to 4 mM, the J SC has hardly any change at all; however, the FF increases 0.412, and as a result, the highest PCE of 1.65% is achieved. The results indicate that the PCE of the devices can be easily improved through a simple Al doping into ZnO lattice process.
where σ was the electrical conductivity, R was the tested value of resistivity, S was the area of the effective measuring electrode, and h was the thickness of the samples. It is found that the σ of AZO whisker samples significantly increased with the increase of Al concentrations . In this study, the value of σ is calculated using the same method, as shown in Table 1. It is found that the σ increases dramatically from 8.2 × 10-5 to 5.1 × 10-4 (Ω cm)-1 with the increase of the Al concentrations from 0 to 4 mM. Compared with the un-doped ZnO nanostructures, the AZO nanostructures can provide a higher conduction pathway to enhance electron transport from P3HT/PCBM matrix to FTO electrodes, as can be clearly clarified in the dark current of devices in Figure 3c. The AZO-based devices have a lower leakage current and R S than that of the un-doped ZnO-based devices. The results are shown in Table 1. Therefore, through increasing the σ of the AZO to facilitate electron transport, the J SC and PCE of IOSCs can be strikingly improved.
In addition, we turn to consider that a suitable morphology of AZO NF array, such as the density of AZO NF arrays, could account for the performance increase in the IOSCs. As is well known, the lowest unoccupied molecular orbital (LUMO) level of ZnO is -4.2 eV and the LUMO level of P3HT is -3.0 eV . It suggests that electrons can be injected from the LUMO of P3HT into the LUMO of ZnO. In this study, upon the Al-doping treatment, it is interesting to observe that the ultrathin and disperse AZO NF arrays have grown on the densely packed ZnO NR array. Generally, the ultrathin and disperse AZO NFs could reach the matrix of P3HT/PCBM, providing a continued "tentacles" for electron collection from PCBM clusters to FTO electrodes. At the same time, owing to the achievement of higher density of AZO NFs, the larger area of interface between AZO NFs and P3HT crystals may induce more sufficient exciton dissociation. The above two factors could explain why the J SC of IOSCs would drop slightly as increasing Al concentration from 2 to 4 mM, even if the σ continues to increase.
To better understand the role of the AZO morphology on the performance of the IOSCs and eliminate the possible effect of different PCBM cluster aggregations on the IOSC performance simultaneously, we fabricated two hybrid solar cells A and B with the structure of FTO/ZnO seed layer/AZO nanostructures/P3HT/Al. The AZO nanostructures, synthesized in a solution of 2 and 4 mM Al concentrations respectively, have a significant variety in morphology, such as the density and the size. The J-V characteristics of the IOSC devices are presented in Figure 3d. It has been found that the σ increases with the increase of Al concentrations from 2 to 4 mM; however, the J SC decreases from 2.73 to 2.37 mA cm-2 and the FF increases from 0.311 to 0.320, and as a result, the PCE decreases from 0.22% to 0.19%. It suggests that less interfacial area between the P3HT and the AZO nanostructures induces a less exciton dissociation, even though AZO nanostructures of a higher σ have been achieved through more Al doping into ZnO lattices. Therefore, a sufficient interface contact for exciton dissociation between P3HT and AZO nanostructures should account for the increase in the PCE of IOSCs.
In conclusion, we fabricated the IOSCs based on the flake-like AZO nanostructures with controllable σ and morphology via a simple hydrothermal method. The effects of the electrical property and morphology characteristics of flake-like AZO nanostructures on the performance of the IOSC devices were investigated. It is found that the PCE of the IOSC devices depends critically on the σ of AZO nanostructures and the interface area between the flake-like AZO nanostructures and the active layer. These results suggest that the flake-like AZO nanostructures could be a promising potential candidate in various photovoltaic and optoelectronic applications to improve device performance.
This work was supported by the National High Technology Research and Development Program of China (2009AA03Z219), 973 Program (no. 2011CB933300) of China, the National Natural Science Foundation of under grant no. 11074194, the Research Program of Suzhou Science & Technology Bureau (SYG201133) and the Fundamental Research Funds for the Central Universities (201120202020001).
- Greene LE, Law M, Yuhas BD, Yang PD: ZnO-TiO(2) core-shell nanorod/P3HT solar cells. J Phys Chem C 2007, 111: 18451. 10.1021/jp077593lView Article
- Liu JP, Wang SS, Bian ZQ, Shan MN, Huang CH: Organic/inorganic hybrid solar cells with vertically oriented ZnO nanowires. Appl Phys Lett 2009, 94: 173107. 10.1063/1.3126955View Article
- Liu NS, Fang GJ, Zeng W, Long H, Fan X, Yuan LY, Zou X, Liu YP, Zhao XZ: Strong Effect of Interelectrode Distance on the Performance of a Novel ZnO Nanorod Lateral Field Emission Device Fabricated by a Single-Step Hydrothermal Approach. J Phys Chem C 2010, 114: 8575. 10.1021/jp1011389View Article
- Shin KS, Lee KH, Lee HH, Choi D, Kim SW: Enhanced power conversion efficiency of inverted organic solar cells with a Ga-doped ZnO nanostructured thin film prepared using aqueous solution. J Phys Chem C 2010, 114: 15782. 10.1021/jp1013658View Article
- Lin Y-Y, Lee Y-Y, Chang LW, Wu J-J, Chen C-W: The influence of interface modifier on the performance of nanostructured ZnO/polymer hybrid solar cells. Appl Phys Lett 2009, 94: 063308. 10.1063/1.3080203View Article
- Wu SJ, Tai QD, Yan F: Hybrid Photovoltaic Devices Based on Poly (3-hexylthiophene) and Ordered Electrospun ZnO Nanofibers. J Phys Chem C 2010, 114: 6197. 10.1021/jp910921aView Article
- Li YJ, Lu MY, Wang CW, Li KM, Chen LJ: ZnGa 2 O 4 nanotubes with sharp cathodoluminescence peak. Appl Phys Lett 2006, 88: 143102. 10.1063/1.2191418View Article
- Wang H, Baek S, Song J, Lee J, Lim S: Microstructural and optical characteristics of solution-grown Ga-doped ZnO nanorod arrays. Nanotechnology 2008, 19: 075607. 10.1088/0957-4484/19/7/075607View Article
- Bae SY, Na CW, Kang JH, Park J: Comparative structure and optical properties of Ga-, In-, and Sn-doped ZnO nanowires synthesized via thermal evaporation. J Phys Chem B 2005, 109: 2526. 10.1021/jp0458708View Article
- Xue XY, Li LM, Yu HC, Chen YJ, Wang YG, Wang TH: Extremely stable field emission from AlZnO nanowire arrays. Appl Phys Lett 2006, 89: 04311.
- Yun SN, Lee J, Yang J, Lim S: Hydrothermal synthesis of Al-doped ZnO nanorod arrays on Si substrate. Physica B 2010, 405: 413. 10.1016/j.physb.2009.08.297View Article
- Zhao DW, Tan ST, Kec L, Liu P, Kyaw AKK, Sun XW, Lo GQ, Kwong DL: Optimization of an inverted organic solar cell. Solar Energy Materials & Solar Cells 2010, 94: 985. 10.1016/j.solmat.2010.02.010View Article
- Miyata N, Akiyoshi S: Preparation and electrochromic properties of RF-sputtered molybdenum oxide films. J Appl Phys 1985, 58: 1651. 10.1063/1.336307View Article
- Julien C, Khelfa A, Hussain OM, Nazri GA: Synthesis and characterization of flash-evaporated MoO 3 thin films. Journal of Crystal Growth 1995, 156: 235. 10.1016/0022-0248(95)00269-3View Article
- Navas I, Vinodkumar R, Lethy KJ, Detty AP, Ganesan V, Sathe V, Mahadevan Pillai VP: Growth and characterization of molybdenum oxide nanorods by RF magnetron sputtering and subsequent annealing. J Phys D: Appl Phys 2009, 42: 175305. 10.1088/0022-3727/42/17/175305View Article
- Huang SP, Xiao Q, Zhou H, Wang D, Jiang WJ: Hydrothermal synthesis and conductive properties of Al-doped ZnO rod-like whiskers. Journal of Alloys and Compounds 2009, 486: L24. 10.1016/j.jallcom.2009.07.033View Article
- Hames Y, Alpaslan Z, Kösemen A, San SE, Yerli Y: Electrochemically grown ZnO nanorods for hybrid solar cell applications. Solar Energy 2010, 84: 426. 10.1016/j.solener.2009.12.013View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.